Piezochromic Porous Metal-Organic Framework.
Andrzejewski, Michał; Katrusiak, Andrzej; The journal of physical chemistry letters 8 (2017) 279–284; doi:10.1021/acs.jpclett.6b02458

data_8000376
_publ_section_title
;
 Piezochromic Porous Metal-Organic Framework.
;
_journal_issue                   1
_journal_name_full               'The journal of physical chemistry letters'
_journal_page_first              279
_journal_page_last               284
_journal_paper_doi               10.1021/acs.jpclett.6b02458
_journal_volume                  8
_journal_year                    2017
_chemical_formula_moiety         'C14 H18 Co N2 O5'
_chemical_formula_sum            'C14 H18 Co N2 O5'
_chemical_formula_weight         353.23
_chemical_name_common            AMU1
_chemical_name_systematic
;
Co(1,4-benzenedicarboxylate)(1,4-diazabicyclo[2.2.2]octane)H2O
;
_space_group_crystal_system      triclinic
_space_group_IT_number           1
_space_group_name_Hall           'P 1'
_space_group_name_H-M_alt        'P 1'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     direct
_audit_creation_date             2016-07-12
_audit_creation_method
;
Olex2 1.2
(compiled 2016.02.19 svn.r3266 for OlexSys, GUI svn.r5155)
;
_cell_angle_alpha                90.369(11)
_cell_angle_beta                 96.279(12)
_cell_angle_gamma                94.712(4)
_cell_formula_units_Z            1
_cell_length_a                   5.9012(3)
_cell_length_b                   7.0666(3)
_cell_length_c                   10.625(3)
_cell_measurement_reflns_used    991
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      55.834
_cell_measurement_theta_min      5.786
_cell_volume                     438.88(13)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXS (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.270
_diffrn_measured_fraction_theta_max 0.246
_diffrn_measurement_device_type  'multiwire proportional'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.2092
_diffrn_reflns_av_unetI/netI     0.1740
_diffrn_reflns_Laue_measured_fraction_full 0.270
_diffrn_reflns_Laue_measured_fraction_max 0.246
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       3
_diffrn_reflns_limit_l_min       -3
_diffrn_reflns_number            2827
_diffrn_reflns_point_group_measured_fraction_full 0.270
_diffrn_reflns_point_group_measured_fraction_max 0.246
_diffrn_reflns_theta_full        26.000
_diffrn_reflns_theta_max         27.917
_diffrn_reflns_theta_min         2.893
_exptl_absorpt_coefficient_mu    0.999
_exptl_absorpt_correction_T_max  0.909
_exptl_absorpt_correction_T_min  0.892
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
Data were collected and reduced by program CrysAlisPro, 
and SCALE3 ABSPACK was used for absorption correction
;
_exptl_crystal_colour            orange/yellow
_exptl_crystal_density_diffrn    1.337
_exptl_crystal_description       plate
_exptl_crystal_F_000             183
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.1
_refine_diff_density_max         1.752
_refine_diff_density_min         -1.695
_refine_diff_density_rms         0.289
_refine_ls_abs_structure_details
;
 Refined as a perfect inversion twin.
;
_refine_ls_abs_structure_Flack   0.5
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   2.143
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     64
_refine_ls_number_reflns         991
_refine_ls_number_restraints     48
_refine_ls_restrained_S_all      2.529
_refine_ls_R_factor_all          0.2813
_refine_ls_R_factor_gt           0.2116
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.2000P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.4565
_refine_ls_wR_factor_ref         0.5278
_reflns_Friedel_coverage         1.000
_reflns_Friedel_fraction_full    0.270
_reflns_Friedel_fraction_max     0.246
_reflns_number_gt                662
_reflns_number_total             991
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            jz6b02458_si_004.cif
_cod_data_source_block           075GPa_P1
_cod_original_cell_volume        438.86(13)
_cod_database_code               8000376
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups
 At 1.5 times of:
  All O(H,H) groups
2. Restrained distances
 O2-C7
 1.25 with sigma of 0.002
 C8-C4
 1.48 with sigma of 0.002
 C1-C7
 1.48 with sigma of 0.002
 C4-C5
 1.38 with sigma of 0.002
 C5-C6
 1.38 with sigma of 0.002
 C6-C1
 1.38 with sigma of 0.002
 C1-C2
 1.38 with sigma of 0.002
 C2-C3
 1.38 with sigma of 0.002
 C3-C4
 1.38 with sigma of 0.002
 C9-N1
 1.46 with sigma of 0.002
 N1-C13
 1.46 with sigma of 0.002
 N1-C11
 1.46 with sigma of 0.002
 C12-N2
 1.46 with sigma of 0.002
 N2-C14
 1.46 with sigma of 0.002
 N2-C10
 1.46 with sigma of 0.002
 C9-C10
 1.52 with sigma of 0.002
 C13-C14
 1.52 with sigma of 0.002
 C11-C12
 1.52 with sigma of 0.002
 O2_$1-C7_$1
 1.25 with sigma of 0.002
 O1_$2-C7_$1
 1.25 with sigma of 0.002
 O4-C8
 1.25 with sigma of 0.002
 O3-C8
 1.25 with sigma of 0.002
 O3-O4
 2.16 with sigma of 0.002
 N1-C9
 1.48 with sigma of 0.002
 N1-C11
 1.48 with sigma of 0.002
 N1-C13
 1.48 with sigma of 0.002
 N2-C14
 1.48 with sigma of 0.002
 N2-C12
 1.48 with sigma of 0.002
 C10-N2
 1.48 with sigma of 0.002
 C9-C10
 1.52 with sigma of 0.002
 C14-C13
 1.52 with sigma of 0.002
 C12-C11
 1.52 with sigma of 0.002
 O1_$2-O2_$1
 2.16 with sigma of 0.002
 C5_$3-C8_$3 \\sim C8_$3-C3_$3
 with sigma of 0.02
 O1_$2-Co1_$2 \\sim Co1_$2-O2_$1
 with sigma of 0.02
 C14-C12 \\sim C12-C10
 with sigma of 0.02
 C9-C13 \\sim C13-C11
 with sigma of 0.02
3. Restrained planarity
 O2, C7, C1, C6, C5, C4, C3, C8, O4, O3, C2
 with sigma of 0.1
4. Uiso/Uaniso restraints and constraints
Uiso(C3) = Uiso(C6) = Uiso(C1) = Uiso(C2) = Uiso(C4) = Uiso(C5) = Uiso(C8)
Uiso(O3) = Uiso(O4) = Uiso(O2) = Uiso(O1)
Uiso(C9) = Uiso(C10) = Uiso(C14) = Uiso(C13) = Uiso(C12) = Uiso(C11)
5.a Rotating group:
 O1W(H1WA,H1WB)
5.b Secondary CH2 refined with riding coordinates:
 C11(H11,H11B), C9(H9A,H9B), C12(H12A,H12), C10(H10A,H10B), C14(H14A,H14B),
 C13(H13A,H13B)
5.c Aromatic/amide H refined with riding coordinates:
 C6(H6), C2(H2), C3(H3), C5(H5)
5.d Fitted hexagon refined as free rotating group:
 C6(C1,C2,C3,C4,C5)
;
_shelx_hkl_checksum              68847
_olex2_submission_special_instructions 'No special instructions were received'